Presented at IMAPS 2014
Photopatternable Laminate BCB Dielectric
Corey OConnor, Robert Barr, Jeff Calvert, Anupam Choubey, Mike Gallagher, Elissei Iagodkine, Joon-
Seok Oh, Andrew Politis, Kevin Wang
Dow Electronic Materials, 455 Forest St, Marlborough, MA 01752 USA
Abstract Divinylsiloxane-bis-benzocyclobutene (DVS-bis-BCB, or BCB) is a well-known dielectric
material that has been used in high volume manufacturing for many years (CYCLOTENE
series Advanced Electronic Resins). Typically, the application of these products has been by spincoating or
spray coating of the dielectric material from a solvent-based formulation. However, for certain applications
- for example, those involving large area, square substrates such as glass panels - it is desirable to be able to
apply the BCB-based dielectric material using a dry film coating process, such as vacuum or hot roll
lamination. In this paper, we describe the concept of creating a laminate film utilizing DVS-bis-BCB as the
primary dielectric material component. In creating the laminate dielectric material, it is important to
maintain the unique combination of thermal and electrical properties of DVS-bis-BCB, including high
thermal stability, excellent copper barrier properties, low moisture uptake, low dielectric constant, and low
dielectric loss. However, DVS-bis-BCB alone is too rigid to produce a high quality laminate film,
therefore, it is necessary to modify the formulation to improve flexibility and lamination quality. As the
flexibility of the film is increased, higher fracture toughness (K1C) and higher elongation values should
result. Novel formulation adjustments to the base DVS-bis-BCB polymer system have resulted in an
experimental laminate dielectric product that will be the focus of this discussion.
Depending on the application, laminate films can vary in thickness from 2m to 50m or even
thicker. A typical laminate film construct includes the BCB-based dielectric film with a base sheet of an
optically-clear polyester (PET) film and a polyethylene (PE) cover sheet. The DVS-bis-BCB-based
laminate can be tuned with appropriate additives to either pattern with UV exposure from a tool such as a
Sss MicroTec Mask Aligner (50mJ/cm2 100mJ/cm
2 exposure energy) or laser pattern with a tool such as
a Sss MicroTec 248nm Excimer Laser. Aspect ratios of 1:1.5 have been achieved with a photopatternable
DVS-bis-BCB film and aspect ratios of >1:1 are possible with a laser-patterned film. Beside the
photopackage added to the film to enable UV patterning, toughening additives have also been incorporated
to enhance the fracture toughness (K1C) and elongation properties. K1C for the laminate has been improved
for DVS-bis-BCB. Elongation has been improved to 13% for the
laminate vs. 8% for DVS-bis-BCB. Electrical properties are similar to DVS-bis-BCB. An additional
attribute of the laminate dielectric is the ability to tent over and protect vias. Vias >100m diameter have
successfully been tented with a 10m thick film. A DVS-bis-BCB-based laminate has been demonstrated
with continued optimization and evaluation to follow.
Key words Dielectric, Benzocyclobutene, Photopatternable, Laser Ablation, Laminate
Panel processing to reduce the cost of packaging electronic
devices for consumer applications is currently the focus of
significant R&D effort in the industry. The adoption of this
technology requires the continued development of
interesting interconnect solutions that reduce the size of
signal routing and, therefore, impose new demands on the
dielectric materials used to isolate the copper interconnects.
Benzocyclobutene polymers have been used to isolate
copper interconnects in packaging applications for more
than 20 years, due in large part to the very low copper drift
rate for this polymer platform [1-4]. In addition, the BCB
platform has a number of other attributes that make it
attractive for new material development including low
dielectric constant, low moisture absorption, rapid low
temperature curing without generation of by-products,
minimum shrinkage in cure process, and proven reliability
[5-8]. However, the relatively low degree of elongation and
inherent stiffness of the BCB platform has limited its use in
stress buffer applications. Therefore, it is highly desirable to
improve the mechanical properties of the polymer platform
while maintaining the good electrical and physical attributes
of BCB polymer, enabling the development of both laser
and photopatternable laminate BCB dielectrics.
II. Overview of Photo and Laser Patternable
Mechanical and Electrical Properties of Dielectric Film
A dielectric film that is BCB-based and both photo and
laser patternable has been developed for next-generation
packaging needs. Toughening additives have enhanced the
mechanical properties of the film while the electrical
properties are similar to BCB.
Table I. BCB Laminate Dielectric Material Properties vs.
Various Dielectrics Material Property
BCB Laminate Dielectric
Polyimide Epoxy/ Phenol
200 - 250 200 - 250 350 190 200 175 - 225
Tg (C) 250 >350 >350 210 180 250
63 42 34 45) vs.
4000 Resin will also yield finer pitch and
higher density lithography.
Figure 1. Cross-section SEM images of vias
photopatterned in the BCB laminate dielectric film
15m Via 20m Via 25m Via
Laser Ablation Patterning of BCB Laminate Dielectric
To evaluate the laser patterning performance of the film, a
10m coating of BCB laminate dielectric was applied to a
silicon substrate, blanket UV exposed (50mJ/cm2), soft
cured (200C for 100mins.), and then ablated with a Sss
MicroTec 248nm Excimer Laser. The ablation energy was
650mJ/cm2 per pulse for 52 pulses. The images below
show that 6m line/space structures with an improved
aspect ratio of 3:1 can be achieved using laser ablation.
Figure 2. 6m line/space pattern in 10m thick film (image
courtesy of Fraunhofer IZM)
Figure 3. Cross-section image of 6m line/space pattern
shown from above in Fig. 2. (image courtesy of Fraunhofer
Fig. 3 above shows that there is some top-loss associated
with the laser ablation process as a 10m film has been
reduced to 9.3m thickness. The laser fluence used has
resulted in a 3.1m trench width for a 3:1 aspect ratio. In
this case, higher resolution is possible when using laser
ablation vs. standard photolithographic processing.
Tenting Performance of BCB Laminate Dielectric
The ability of the BCB laminate dielectric to tent and
protect vias having a diameter of at least 100m is unique to
this format as compared to a spin-on dielectric that will not
have the ability to span openings present on glass or silicon
substrates. The following images show a 10m film applied
over 100m vias with hot roll lamination. The film was
processed through hard cure (250C for 60mins.) with no
degradation or openings in the tents.
Figure 4. BCB laminate dielectric applied over 100m vias
Figure 5. Magnified image of BCB laminate dielectric
applied over 100m via
An advantage of the tenting ability of the film as compared
to a standard spin-on resist is the ability to exclude plating
from non-conductive vias.
III. BCB Laminate Dielectric Construction
Figure 6. BCB laminate dielectric on plastic core
Figure 7. BCB laminate dielectric film construction
As this is a thin film coating, high quality polyethylene is
used as a cover sheet to prevent gels from imprinting holes
or voids into the coating. Optically clear polyester is also
critical as exposing radiation will be passing through the
backsheet and distortion should be limited.
IV. Processing Conditions for BCB Laminate
Table III. Processing Conditions of BCB Laminate
Dielectric vs. CYCLOTENE
3000/4000-Series Dielectrics Process Step BCB Laminate Dielectric CYCLOTENE
Adhesion Promoter Current version self-priming AP3000
Application Hot roll or vacuum laminator Spin-coated
Post-Application Bake Step Not Required 90C/90s (assume 10m tks)
Thickness 5 - 50m 1 - 15m
Exposure Type and Energy i-line or Broadband (BB), exposure depending on film
thickness (50mJ/cm2 for 10m film)
i-line or BB, exposure depending on film thickness
Post-Exposure Bake 90C/90s 80C/90s
Develop Puddle or spray with Dows DS2100 solvent developer
Post-Develop Bake 90C/60s Spin dry
Hardcure 250C/60min. in Nitrogen-purged environment
Table III summarizes the processing conditions for the BCB
laminate dielectric as compared to the CYCLOTENE
Substrate Surface Preparation
The current version of the laminate is self-priming. For
some applications, an adhesion promoter designed for use
with BCB-based dielectrics such as Dows AP9000M or
AP9000S may be used, if needed. Prior to film lamination,
the adhesion promoter is applied to the substrate by
dispensing either statically or dynamically. The substrate is
then spun dry at 2000rpm for 10- 20s and baked to remove
the solvent carrier for 30sec. at 90-150C.
The film may be applied by hot roll lamination with a tool
such as the Western Magnum XRL-120 Hot Roll
Laminator. The polyethylene cover sheet is peeled away
while the BCB laminate dielectric is adhered to the
substrate surface at a speed of 2fpm and a temperature of
107C. The polyester backsheet is left to cover the laminate
coating through exposure for protection against both
physical damage and oxygen inhibition during free radical
polymerization. Vacuum lamination is another possible
method of applying the BCB laminate dielectric.
Advantages of a BCB laminate dielectric versus a spin-on
coating include enhanced thickness control, availability of
multiple film thicknesses with the ability to coat very thick
layers, and the absence of a baking step to eliminate solvent.
This results in a lower VOC process.
Exposure and Post-Exposure Bake
In this description, the Sss MicroTec Mask Aligner was
used to cure the film. Exposure energy will depend on film
thickness. At a film thickness of 10m, 50mJ/cm2 was
sufficient to cure the film. A 90C/90s bake step is used
post-exposure to complete the free radical polymerization.
Development and Post-Develop Bake
Dows DS2100 Solvent Developer was used to dissolve the
unexposed portions of the film and create the intended
pattern. In this description, a puddle develop step of 180s
was used which was followed by a spin step at 1000rpm to
remove the dissolved portions while spraying with fresh
developer to clean out finer features. A final 2000rpm spin
step is used to remove the developer. To dry the wafer, a
post-develop bake step of 90C for 60s is used.
As an alternative to UV exposure and development, laser
ablation can be used as a means to open features in the
laminate dielectric. A Sss MicroTec 248nm Excimer
Polyethylene Cover Sheet
BCB Laminate Dielectric
Laser was used with an exposure energy of 650mJ/cm2 per
pulse and requiring 52 pulses to transfer the pattern. For
this experiment, a 5m sacrificial layer was applied over the
laminate dielectric to capture particles produced by the
ablation process. Post-ablation, the sacrificial layer was
stripped to reveal a clean, patterned layer.
BCB Curing Step
Post-patterning, the laminate can be either soft cured at
200C for 100min or hard cured at 250C for 60min,
depending on the amount of BCB polymerization required.
The laminate is oven-cured in an N2 atmosphere as BCB is
susceptible to oxidation at elevated temperatures.
This paper summarizes the development of a BCB-based
laminate dielectric with performance advantages as
compared to CYCLOTENE
and other current dielectric materials. Improved mechanical
properties, similar electrical properties, and the ability to
tent vias are seen as properties suited for the next generation
of electronic devices. Enhanced lithographic resolution and
faster photospeed are additional benefits that will enable
higher density patterns and faster manufacturing throughput.
Laminate products demonstrate the ability for improved
thickness control, the introduction of a wide range of
available thicknesses, and the exclusion of VOC-producing
steps such as the bake process following liquid dielectric
application. Further processing advantages can be realized
when laser patterning is employed, including improved
resolution and the elimination of UV exposure and
We would like to thank Dr. Jong-Uk Kim of Dow Advanced
Packaging Technologies and Dr. Michael Tpper of
Fraunhofer IZM for support in laser patterning of BCB-
laminate dielectric material.
Trademark of The Dow Chemical Company (Dow) or an affiliated company.
 Burdeaux, D.; Townsend, P.; Carr, J.; Garrou, P.,
Benzoclybutene (BCB) dielectrics for the fabrication of
high-density, thin-film multichip modules. Journal of
Electronic Materials 1990, 19 (12), 1357-1364.
 Kirchhoff, R. A.; Carriere, C. J.; Bruza, K. J.; Rondan,
N. G.; Sammler, R. L., Benzocyclobutenes - a new class of
high-performance polymers. Journal of Macromolecular
Science-Chemistry 1991, A28 (11-12), 1079-1113.
 Loke, A. L. S.; Wetzel, J. T.; Townsend, P. H.; Tanabe,
T.; Vrtis, R. N.; Zussman, M. P.; Kumar, D.; Ryu, C.;
Wong, S. S., Kinetics of copper drift in low-kappa polymer
interlevel dielectrics. IEEE Transactions on Electron
Devices 1999, 46 (11), 2178-2187.
 Mills, M. E.; Townsend, P.; Castillo, D.; Martin, S.;
Achen, A., Benzocyclobutene (DVS-BCB) polymer as an
interlayer dielectric (ILD) material. Microelectronic
Engineering 1997, 33 (1-4), 327-334.
 Bothra, S.; Kellam, M.; Garrou, P., Feasibility of BCB
as an interlevel dielectric in integrated-circuits. Journal of
Electronic Materials 1994, 23 (8), 819-825.
 Garrou, P. E.; Heistand, R. H.; Dibbs, M. G.; Mainal,
T. A.; Mohler, C. E.; Stokich, T. M.; Townsend, P. H.;
Adema, G. M.; Berry, M. J.; Turlik, I., Rapid thermal
curing of BCB dielectric. IEEE Transactions on
Components Hybrids and Manufacturing Technology 1993,
16 (1), 46-52.
 Johnson, R. W.; Phillips, T. L.; Weidner, W. K.; Hahn,
S. F.; Burdeaux, D. C.; Townsend, P. H., Benzocyclobutene
interlayer dielectrics for thin-film multichip modules. IEEE
Transactions on Components Hybrids and Manufacturing
Technology 1990, 13 (2), 347-352.
 So, Y. H.; Garrou, P.; Im, J. H.; Scheck, D. M.,
Benzocyclobutene-based polymers for microelectronics.
Chemical Innovation 2001, 31 (12), 40-47.